Biswajit Bera / International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 2, Issue 5, September- October 2012, pp.404-411

Adhesional Friction Law and Adhesive Wear Law of Micromechanical Surface Contact Biswajit Bera* *(Department of Mechanical Engineering, National Institute of Technology Durgapur, India)

1. Introduction Friction could be defined as the force of resistance that occurs when one body moves tangentially over another body. In the 15th century da Vinci discovered a law about dry sliding friction, which was rediscovered by Amontons about 200 years later. Friction laws were stated by French engineer Guillaume Amontons [1] in 1699 from the conclusions of his experimental work which are given as follows: a)

The friction force linearly proportional to the normal load between the two bodies in contact. b) The friction force is independent of the apparent area of contact between the two bodies. Thereafter, microscopic analysis of friction process was described by Bowden and Tabor [2] in 1931. The theory was based on following two statements: a)

The friction force is dependent on real area of contact between two bodies. b) The friction force is dependent on shearing strength of adhesive bond formed between two bodies at tip of asperities. The adhesional friction theory of Bowden and Tabor is appeared to be inconsistent with Hertz theory of deformation of contacting elastic asperities, which predicts that the contact area should vary as 2/3

power of load  P  

 Ka 3  a 2  P 2/ 3  .To avoid R 

the violation of the theory, Bowden and Tabor simply, mentioned that all asperities should deform plastically and real area of contact is linearly

404 | P a g e

Biswajit Bera / International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 2, Issue 5, September- October 2012, pp.404-411 asperities due to localized high adhesion and the subsequent shearing of the junctions from weaker material causing adhesive wear. Similar idea is implemented to find new adhesive wear law considering adhesion component of JKR adhesion model [3]. Thereafter, it is compared with existing Archard's adhesive wear law.

 G 4 K

 G

 3 R 

  3 R 

0

2KR

2

2

1.5 1.5

(3)

where 1  2  1  1  2

2. Single asperity contact

G

2.1 Single asperity real area of contact JKR adhesion theory has modified Hertz theory of spherical contact. It predicts a contact radius at light loads greater than the calculated Hertz radius. As asperity tip is considered spherical, the adhesion model of single asperity contact could be extended to multiasperity of rough surface contact. So, real contact area of single asperity is

2 RF

4 K

Ta 

G2

2.4 Single asperity adhesive wear volume If wear particle is in the shape of hemispherical and is cut off from tip of the asperity, wear volume is 2 Va  a 3 3

2

R 3 A a   F0  3 R  6 RF0  (3 R ) 2  K  

G1

2 R   F0  3 R  6 RF0  (3 R ) 2  3  K 

Substituating F  K (R) , we get 0 1.5

Substituting F  K (R) , we get a 1.5

R

R

 3 R 2 6 R 3.5 1.5 9 2  2 R 4  A a  R 1.5 1.5     K K K 2  

2 3

Va 

(1)

  

(4)

3. Multiasperity contact

2.2 Single asperity adhesional loading force According to JKR adhesion model, the expression of adhesional loading force for each asperity contact is Fa  F0  3 R  6 RF0  (3 R ) 2  KR 0.5 1.5  3R  6KR1.5 1.5  (3R) 2

2  1.5 1.5 3 R 2 6 R 3.5 1.5 9 2  2 R 4 R     3  K K K2

(2)

where 1  3  1 12  1  22  K 4  E1 E 2  and E1 , E2 ,  1 and  2 are Young’s modulus and poisson’s ratios of the contacting surfaces respectively,

First of all, Greenwood and Williamson [8] developed statistical multyasperity contact model of rough surface under very low loading condition and it was assumed that asperities are deformed elastically according Hertz theory. Same model is modified here in adhesive rough surface contact and it is based on following assumptions: i. ii. iii. iv. v. vi.

The rough surface is isotropic. Asperities are spherical near their summits. All asperity summits have the same radius R but their heights vary randomly. Asperities are far apart and there is no interaction between them. Asperities are deform elastically according to JKR adhesion theory There is no bulk deformation. Only, the asperities deform during contact. Flat plane

where surface energy of both surfaces,   1   2  12 2.3 Single asperity adhesional friction force

δ Savkoor and Briggs theory has found adhesional friction of spherical contact under tangential loading. As asperity tip is considered spherical, the adhesional friction model of single asperity contact could be extended to multiasperity of rough surface contact. According to the Savkoor and Briggs model, the expression of adhesional friction force for each asperity contact is

d

Z

Mean Rough surface

Fig. 1 Rough surfaces contact

405 | P a g e

Biswajit Bera / International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 2, Issue 5, September- October 2012, pp.404-411 Multiasperity contact of adhesive rough surface has shown in Fig.1. According to, GW model, two rough surface contact could be considered equivalently, contact between rough surface and smooth rigid surface. Let z and d represents the asperity height and separation of the surfaces respectively, measured from the reference plane defined by the mean of the asperity height. δ denotes deformation of asperity by flat surface. Number of asperity contact is 

N c  N  ( z )dz

0.5   R    (  R  )  3(R)         K    * F   ()d 0.5 2 0  6(R) 2    R  1.5  9 2 (R) 2       K     K  

0 R 00.5  3A 0 B0   1  h   2     exp d 2 0.5 1.5 2 2 2 2  0    6A 0 B0 R 0   9 A 0 B0  2 

(5)

d

where N is total number of asperity and  (z ) is the Gaussian asperity height distribution function. 3.1 Multiasperity real area of contact

where dimensionless surface roughness parameter, A 0  R and dimensionless surface energy parameter, B0  

K

n

So, from eq (1) and (5), real area of contact for multiasperity contact is

So, , from eqn (3) and (5), total adhesional friction force for multiasperity contact is

A  N  A a ( z )dz

T  N c Ta

d

  N   d 

2

 3 R 2 6 R 3.5 1.5 9 2  2 R 4  3  N  R 1.5 1.5     (z)dz K K K 2   d  

Dividing both side by apparent area of contact An

0.5  1.5  1.5 1.5 2.5 1.5    R      (R)   3 (R)   K         A*     ()d 0.5 2 0   R  R         1.5 5 3 6  4 (  R) 3    9  (  R  )         K     K      

 1.5 A1.5 1.5  3 2.5 A1.5 B R 0.5   1  h   2  0 0 0 0    exp d 4 3 0.5 1.5 5 3 2 2  0   6 A 0 B0 R 0   9 A 0 B0 R 0  2

 G

2 KR

 2   3 R  (z)dz  

1.5 1.5

Dividing both side by AnK  T    0  

4 K

*

    0 

4 K

4 K

 G

 G

   R  2(R)     K    2

0.5

2       3 (R)   ()d  K    1.5

2

2

  h   2  1 2A 02 B0 R 0 0.5 1.5  3 2 A 02 B02  exp   d  2 2   

3.4 Multiasperity adhesive wear volume So, from eqn (4) and (5), adhesive wear volume for multiasperity contact is V  N c Va

F Nc Fa

 N  KR 0.5 1.5  3 R  6 KR 1.5 1.5  (3 R ) 2 (z)dz

 N  Va (z)dz d

d

Dividing both side by AnK

 2  3 R 2 6 R 3.5 1.5 9 2  2 R 4   N  R 1.5 1.5     (z)dz 3  K K K 2  d

Dividing both side by A n 

406 | P a g e

0.5    R  1.5    R  (  R  )   3(R)           K    2   * V    ()d 1.5 2 2 3 0  R  R   1.5     2 2  6(R) 2      9 (R)       K     K     

0.5 1.5  1  h   2  2 A 0 R 0   3A 0 B0 R 0      exp  d 2 1 . 5 1 . 5 2 2 2 2 3 0  6A 0 B0 R 0   9 A 0 B0 R 0  2 2     

4. Results and Discussion

4.1 Investigation on adhesional friction law ROUGH

SMOOT H

INT ERMEDIAT E

SUPER SMOOT H

REAL AREA OF CONTACT (A * )

0.90 0.80 0.70 0.60 0.50 0.40 0.30 0.20 0.10 0.00 3

2

1

0

MEAN SEPARAT ION (h)

Fig.2 Real area of contact

-1

ROUGH

SMOOT H

INT ERMEDIAT E

SUPER SMOOT H

0.003 0.002 0.002 0.001 0.001 0.000 4

Tayebi and Polycarpou [9] have done extensive study on polysilicon MEMS surfaces and four different MEMS surface pairs. Similarly, tribological properties of the MEMS surfaces are being considered for present study as input data as shown in table 1 [Appendix A].The material properties of MEMS surface samples are modulus of elasticity, K =4/3E = 112 GPa, modulus of rigidity, G = 18.42 GPa hardness, H = 12.5 GPa, and poisions ratio, ν1 = ν2 = 0.22

4

Biswajit Bera / International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 2, Issue 5, September- October 2012, pp.404-411

3

2

1

0

MEAN SEPARAT ION (h)

407 | P a g e

-1

ROUGH

SMOOT H

ROUGH

SMOOT H

INT ERMEDIAT E

SUPER SMOOT H

INT ERMEDIAT E

SUPER SMOOT H

AREA COEFFICIENT OF FRICTION (T * /A* )

AREA COEFFICIENT OF LOAD (F * /A* )

Biswajit Bera / International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 2, Issue 5, September- October 2012, pp.404-411

0.08 0.07 0.06 0.05 0.04 0.03 0.02 0.01 0.00 4

3

2

1

0

0.02 0.01 0.01 0.01 0.01 0.01 0.00 0.00 0.00

-1

4

3

MEAN SEPARAT ION (h)

2

1

0

-1

MEAN SEPARAT ION (h)

Fig.4 Area coefficient of load Fig.6 Area coefficient of friction Fig.4 shows area coefficient of load verses dimensionless mean separation. This coefficient is considered to understand the relationship in between real area of contact and loading force. Generally, it is assumed that real area of contact and load are linearly proportional as mentioned by Bowden and Tabor considering plastic deformation of asperity. For mean separation smaller than 1, area coefficient for all four cases are comparatively small and are of the slightly descending with same magnitude. However, as mean separation larger than 2, deviation in the coefficient among the four cases becomes increasing prominent and it maintain almost different constant value with mean separation. The separation in between 2 and 1, there is transition of the coefficient from higher different value to lower descending constant value. So, from the discussion, it is found that it do not support the linear relationship in between real area of contact and the loading force SMOOT H

*

INT ERMEDIAT E

Fig.6 shows area coefficient of friction verses dimensionless mean separation and it follows the similar nature of curve as shown for area coefficient of the loading force. Similarly, It shows non linear relationship in between real area of contact and friction force.

COEFFICIENT OF FRICTION (T * /F* )

ROUGH

From Fig.5, adhesional friction force increases with decrement of dimensionless mean separation exponentially. It is found that maximum adhesional friction force for the all MEMS surfaces increases as smoothness of MEMS surface increases. Adhesional friction force for super smooth MEMS surface is very high due to presence of strong attractive adhesive force. On the other hand, adhesional friction force is very small for the rough MEMS surface contact.

SUPERSMOOT H

0.0008 0.0007 0.0006 0.0005 0.0004 0.0003 0.0002 0.0001

ROUGH

SMOOT H

INT ERMEDIAT E

SUPER SMOOT H

0.50 0.45 0.40 0.35 0.30 0.25 0.20 0.15 0.10 0.05 0.00 4

3

2

1

0

-1

MEAN SEPARAT ION (h)

0.0000 4

3

2

1

MEAN SEPARAT ION (h)

0

-1

Fig.7 Coefficient of friction Fig.7 displays variation of coefficient of friction with mean separation. It is found that static coefficient of friction is almost constant except for

408 | P a g e

Biswajit Bera / International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 2, Issue 5, September- October 2012, pp.404-411

AREA COEFFICIENT OF WEAR (V * /A* )

the super smooth MEMS surface. So, the Amontons law of static friction is validated for adhesive micromechanical surface contact. Only for the supersmooth MEMS surface contact, coefficient of static friction suddenly drops at close contact though nature of curve of adhesional loading force and adhesional friction force for supersmooth MEMS surface is same. 4.2 Investigation on adhesive wear law ROUGH

SMOOT H

INT ERMEDIAT E

SUPER SMOOT H

100.00 90.00

ROUGH

SMOOT H

INT ERMEDIAT E

SUPER SMOOT H

160.00 140.00 120.00 100.00 80.00 60.00 40.00 20.00 0.00 4

80.00

3

2

1

0

MEAN SEPARAT ION (h)

70.00 60.00

Fig.9 Area coefficient of wear

50.00 40.00

* So, Area coefficient of wear  V  V  K adh *

30.00

A

20.00 10.00

A

 V  K adh A

0.00 4

3

2

1

0

-1

MEAN SEPARAT ION (h)

Where real area of surface contact, A  P according H

to Bowden and Tabor theory Fig.8 Adhesive wear volume Fig.8 depicts variation of adhesive wear volume with mean separation. It is found that maximum adhesive wear volume for the all cases of MEMS surfaces increase as smoothness of MEMS surfaces increase. So, super smooth MEMS surface produces maximum adhesive wear volume whereas rough MEMS surface produces very low adhesive wear volume. Fig.9 shows area coefficient of wear verses dimensionless mean separation. This coefficient is considered to understand the relationship in between real area of contact and wear volume. From the nature of curves, it is found that dimensionless adhesive wear volume is almost linearly proportional with dimensionless real area of contact. So area coefficient of wear is almost constant.

P  H

Where V= Wear volume, Kadh = adhesive wear coefficient (i.e. area coefficient of wear), P = normal load, H = soft material hardness, σ = rms roughness of surface. According to new adhesive wear law, adhesive wear coefficient increases with increment of MEMS surface contact. And Kadh = 0.25 for rough surface, Kadh = 5 for smooth surface, Kadh = 30 for intermediate surface, and Kadh = 120 for super smooth surface. .

Now, wear rate, × RPS

v  v × no. of pass per revolution  v  n p  RPS

Generally, Pin on Disk tester are commonly used to measure wear rate. If circular cross sectional pin of diameter, d is placed on disk at diameter, D, no. of pass per revolution, np 

Total area crossed Cross sec tional area of pin

Dd D 4 d d 2 / 4

409 | P a g e

-1

Biswajit Bera / International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 2, Issue 5, September- October 2012, pp.404-411 However, in comparison of new adhesive wear law with Archard's law of adhesive wear, the new law is much more appropriate from the point view of volume concept. In case of well accepted Archard's law of adhesive wear, sliding distance is on the plane of real area of contact and so, how does multiplication of both the two parameter produce volume whereas in case of new law of adhesive wear, r.m.s. roughness perpendicular to the plane of real area of contact which produces volume removal in the form of adhesive wear.

References [1]

G Amontons, Histoire de l'Académie Royale des Sciences avec les Mémoires de Mathématique et de Physique (1699)

[2]

F P Bowden and D Tabor, The Friction and Lubrication of Solids (Oxford University Press, New York 1950)

[3]

K L Jhonson, K Kendall, and A D Roberts, Surface energy and the contact of elastic solids, Proc. R. Soc. Lond., A 324, 1971, 301-313

[4]

B V Derjaguin, V M Muller, and YU P Toporov, Effect of contact deformation on the adhesion of particles, J. Coll. and Inter. Sc., 53, 1975, 314-326

[5]

W R Chang, I Etsion, and D B Bogy, Adhesion model for metallic rough surfaces, Journal of Tribology, 110, 1988, 50-56

[6]

S K Roy Chowdhury and P Ghosh, Adhesion and adhesional friction at the contact between solids, Wear, 174, 1994, 919

[7]

A R Savkoor and G A D Briggs, The effect of tangential force on the contact of elastic solids in adhesion Proc. R. Soc. Lond., A 356, 1977, 103-114

d) Similarly, real area of contact and static adhesional friction force are also nonlinearly proportional.

[8]

J A Greenwood, and J B P Williamson, Contact of nominally flat surfaces. Proc. R. Soc. Lond., A 295, 1966, 300-319

e)

Static coefficient of friction is almost constant for micromechanical surface contact which is theoretical evidence of Amonton's law of friction.

[9]

N Tayebi and A A Polycarpou, Adhesion and contact modeling and experiments in microelectromechanical systems including roughness effects, Microsyst. Technol., 12, 2006, 854-869

f)

Justified new adhesive wear law developed where adhesive wear volume equal to multiplication of real area contact and rms roughness. Coefficient adhesive wear increases as smoothness surface increase.

[10]

B Bera, Adhesion and adhesional friction of micromechanical surface contact. Journal of Engineering and Applied Sciences, 6, 2011, 104-108

[11]

J F Archard, Contact and rubbing of flat surfaces. Journal of Applied Physics, 24, 1953, 981-988

5. Conclusions The study is the theoretical investigation on existing static friction coefficient and adhesive wear law. From the study of micromechanical contact of MEMS surfaces, following conclusions could be drawn: a) When micro-rough surfaces are come in contact due to application of external force, spherical tip of the contacting asperities form adhesive bond followed by JKR adhesion theory. b) As smoothness of surfaces increase, it produces much more strong adhesive bond at the tip of the contacting asperities. c)

Real area of contact increases with adhesional loading force nonlinearly which is generally, considered linearly proportional as stated by Bowden and Tabor.

is is of of of

g) Finally, though above study is done for micro-rough surface contact of MEMS but it could be applicable for macroscopic study of tribo-system as interface is always microscopic.

Acknowledgements I would humbly thank to Prof. B Halder, NIT Durgapur, India whose inspiration and support have made the work successful.

410 | P a g e

Biswajit Bera / International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 2, Issue 5, September- October 2012, pp.404-411 APPENDIX A Table.1 Input data Combined MEMS Surfaces

Rough

Smooth

Intermidiate

Super Smooth

η (m-2)

14.7.1012

11.1. 1012

17.1012

26.1012

R (m)

0.116.10-6

0.45.10-6

1.7.10-6

26.10-6

σ (m)

15.8.10-9

6.8.10-9

1.4.10-9

0.42.10-9

γ (N/m)

0.5

0.5

0.5

0.5

K (N/m2)

112.109

112.109

112.109

112.109

G (N/m2)

18.42.109

18.42.109

18.42.109

18.42.109

A0

27.10-3

34.10-3

41.10-3

53.10-3

B0

2.825.10--4

6.565.10--4

31.887.10--4

74.405.10—4

R0

7.342

66.176

1214.285

5600.000

411 | P a g e